|Year : 2021 | Volume
| Issue : 3 | Page : 128-131
Abutment Screw Loosening in Single Implant Restorations: Evaluation of Fracture Strength of Implant-Supported Cement-Retained Monolithic Zirconia Restorations Repaired with Porcelain and Composite Resin
Hamid Neshandar Asli1, Mehran Falahchai2, Samiye Rahimabadi3, Hamidreza Arbab4, Zoheir Mousavi Mehr2
1 Professor, Dental Sciences Research Center, Department of Prosthodontics, School of Dentistry, Guilan University of Medical Sciences, Rasht, Iran
2 Assistant Professor, Dental Sciences Research Center, Department of Prosthodontics, School of Dentistry, Guilan University of Medical Sciences, Rasht, Iran
3 Dental Sciences Research Center, School of Dentistry, Guilan University of Medical Sciences, Rasht, Iran
4 Assistant Professor, Dental Sciences Research Center, Department of Prosthodontics, School of Dentistry, Alborz University of Medical Sciences, Karaj, Iran
|Date of Submission||21-Apr-2021|
|Date of Decision||16-May-2021|
|Date of Acceptance||16-Sep-2021|
|Date of Web Publication||2-Nov-2021|
Zoheir Mousavi Mehr
Department of Prosthodontics, Dental Sciences Research Center, School of Dentistry, Guilan University of Medical Sciences, Rasht-Fooman Road, Rasht, Postal Code 41938-33697
Source of Support: None, Conflict of Interest: None
Aim: To assess the fracture strength of repaired implant-supported cement-retained monolithic zirconia restorations with porcelain and composite resin. Materials and methods: Nighty monolithic zirconia crowns were cemented over the implant abutments, and divided into three groups (n = 30): control, screw access hole preparation in the crown and its restoration with composite resin (HC), and screw access hole preparation in the crown and its restoration with feldspathic porcelain (HP). Fracture strength was measured by a universal testing machine. Data were analyzed (α < 0.05). Results: The maximum fracture strength was in the control group (764.23 ± 108.41 N), whereas the minimum was in HC group (686.25 ± 101.86 N). The mean fracture strength in HC group was significantly lower than that in the control group (P = 0.008). No significant difference was noted between other groups (P > 0.05). Conclusion: Repaired implant-supported monolithic zirconia crowns with feldspathic porcelain provided a fracture strength comparable to that in the control group.
Keywords: Implant supported dental prosthesis, single-tooth implants, Y-TZP ceramic
|How to cite this article:|
Asli HN, Falahchai M, Rahimabadi S, Arbab H, Mousavi Mehr Z. Abutment Screw Loosening in Single Implant Restorations: Evaluation of Fracture Strength of Implant-Supported Cement-Retained Monolithic Zirconia Restorations Repaired with Porcelain and Composite Resin. Dent Hypotheses 2021;12:128-31
|How to cite this URL:|
Asli HN, Falahchai M, Rahimabadi S, Arbab H, Mousavi Mehr Z. Abutment Screw Loosening in Single Implant Restorations: Evaluation of Fracture Strength of Implant-Supported Cement-Retained Monolithic Zirconia Restorations Repaired with Porcelain and Composite Resin. Dent Hypotheses [serial online] 2021 [cited 2021 Nov 29];12:128-31. Available from: http://www.dentalhypotheses.com/text.asp?2021/12/3/128/329757
| Introduction|| |
Implant-supported fixed restoration is a predictable treatment option which has gained high popularity as a standard treatment., The abutment screw loosening is among the most common complications of implant treatment., Implant crowns may be cement retained or screw retained. Cement-retained crowns have advantages such as the ability to compensate for the improper inclination of implant, passive fit, and allowing occlusal adjustment due to the presence of an intact occlusal surface. However, in the case of abutment screw loosening, they are often damaged to access the abutment screw. Krishnan et al. and Patil suggested reuse of crowns after repairing the screw access hole prepared due to abutment screw loosening, to save time and cost.
Several studies have evaluated the effect of screw access channel preparation on fracture strength of zirconia in screw–cement-retained restorations., Nonetheless, the fracture strength of cement-retained monolithic zirconia crowns after access hole preparation for tightening of a loose abutment has not been investigated. Furthermore, to the best of the authors’ knowledge, repair of screw access holes with porcelain in zirconia crowns has not been previously studied. Thus, this study aimed to assess the fracture strength of implant-supported cement-retained monolithic zirconia restorations repaired with porcelain and composite resin following abutment screw loosening and subsequent screw access hole preparation. The null hypothesis was that the fracture strength of crowns after repair with porcelain and composite resin would not be significantly different from each other and from the fracture strength of intact crowns.
| Materials and Methods|| |
Nighty straight abutments (935729, SIC Standard Abutments, SIC Invent AG, Basel, Switzerland) were fixed on the analogs (5 × 11.5 mm; SIC Lab Implant, SIC Invent AG) according to the manufacturer’s instructions. The analog–abutment assembly was mounted in an acrylic resin mold (Palapress Vario, Heraeus Kulzer, Wehrheim, Germany) at 90° angle relative to the horizon using a surveyor such that the abutment–analog connection was 1 mm above the acrylic surface.
One abutment was scanned by a laboratory scanner (Ceramill Map 400; Amann Girrbach, Koblach, Austria). A full-contour crown was designed for the maxillary first premolar using a software program (Ceramill Mind; Amann Girrbach) and sent to Ceramill milling machine (Motion 2(5×); Amann Girrbach). Nighty monolithic zirconia crowns with 2 mm occlusal thickness were fabricated (Zolid FX multilayer; Amann Girrbach), and sintered according to the manufacturer’s instructions. Eventually, the crowns were cemented (Panavia F2.0; Kuraray Medical Inc, Tokyo, Japan). All specimens underwent 5000 thermal cycles between 5°C and 55°C with a dwell time of 60 seconds and a transfer time of 12 seconds.
A silicon index was obtained for standardization of the final repaired crowns. Thirty specimens were assigned to the control group and remained intact. In the remaining specimens, a taper round-end diamond bur (ZR Diamond, Komet Besigheim, Germany) was used to manually create a hole in the middle of the occlusal surface. A new bur was used for preparation of each specimen. To standardize the holes, a metal index was used. The specimens were then divided into two groups.
Holes restored with composite resin (HC group): The holes were sandblasted with an intraoral sandblaster (Dento-Prep, Ronvig, Daugaard, Denmark) by using 50 μm alumina particles with 40 psi pressure at 10 mm distance for 10 seconds, and then rinsed with water spray for 20 seconds, and dried with air spray for 5 seconds. To create a 2-mm space for the restorative material, a piece of sterile polytetrafluoroethylene (PTFE) tape was placed in the prepared hole, and condensed with a plugger. One layer of Z-Prime Plus primer (Bisco, Schaumburg, Illinois, USA) was applied in the hole and air-dried for 5 seconds. The hole was then restored with composite resin (Filtek Z250; 3M ESPE, St Paul, Minnesota, USA), and cured for 20 seconds using a light-emitting diode device (Elipar Freelight 2; 3M ESPE).
Holes restored with porcelain (HP group): The abutment screw was completely unscrewed, and the crowns were removed along with the abutment and abutment screw. To separate the crowns from the abutment, the specimens were placed in a furnace and heated at 300°C to 400°C, and after 5 minutes of holding time, they were cooled at room temperature. This led to cement degradation. The residual cement on the abutment was removed with acetone and water, and the abutment was dried. The hole was sandblasted as explained earlier. The specimens were ultrasonicated in distilled water at room temperature for 1 minute. Eventually, the created holes were restored with incremental application of feldspathic porcelain (Vita Zahnfabrik, Bad Sackingen, Germany) and baked in two layer according to the manufacturer’s instructions. The crown surface was then polished with diamond discs, and heated again in a furnace at 920°C for 1 minute.
The crowns were cemented again by Panavia F2.0 resin cement (Kuraray Medical Inc) [Figure 1]. Eventually, all specimens were incubated at 37°C and 100% humidity for 24 hours and were then thermocycled again as explained earlier. Next, they underwent fracture strength test in a universal testing machine (DBBP-2t; Bongshin Loadcell Co., Ltd, Seoul, Korea). For this purpose, compressive load was applied by an applicator with 6 mm diameter at a crosshead speed of 1 mm/min with 0° angle relative to the abutment.
The Shapiro–Wilk test showed normal distribution of data in all groups. Thus, one-way analysis of variance (ANOVA) was applied to compare the fracture strength of the groups. Pairwise comparisons were performed by the Tukey post-hoc test at 0.05 level of significance. All statistical analyses were performed by using SPSS version 24 (SPSS Inc., Chicago, Illinois, USA).
| Results|| |
The ANOVA revealed a significant difference in fracture strength of the groups (P = 0.009, F = 5.011). The mean fracture strength was 764.23 ± 108.41 N in the control group, 686.25 ± 101.86 N in HC group, and 709.61 ± 81.47 N in HP group. Pairwise comparisons by the Tukey test showed no significant difference between the HP and control (P = 0.100) or HP and HC (P > 0.999) groups. However, the fracture strength of HC group was significantly lower than that of the control group (P = 0.008) [Table 1].
| Discussion|| |
The current results revealed a significant difference in the mean fracture strength of the groups. Thus, the null hypothesis of the study was rejected.
In this study, preparation of access holes in implant-supported cement-retained monolithic zirconia crowns and their repair with composite resin significantly decreased their fracture strength. This result was in line with Wood et al., Scioscia et al., and Mokhtarpour et al. It should be noted that preparation of sintered zirconia decreases its mechanical properties, and the zirconia strength is directly affected by the size, number and location of cracks such that the superficial cracks directly serve as areas of stress accumulation, and can aggravate the stress depending on their size.
According to the results of the present study, preparation of monolithic zirconia crowns and repair of the cavity with porcelain did not significantly decrease the fracture strength of implant-supported crowns. Although the bond strength between the veneering porcelain and zirconia has been previously studied,,, to the best of the authors’ knowledge, repair of cavities prepared in monolithic zirconia with feldspathic porcelain has not been previously investigated. It is believed that the bonding of porcelain to zirconia restorations is influenced by formation of oxide layer, mechanical bonding by sandblasting, and compressive bonding due to the difference in the coefficients of thermal expansion. However, the details of these mechanisms have yet to be clearly elucidated. The bond between the porcelain and zirconia may be influenced by residual thermal stresses in the cooling phase. Thus, most manufacturers produce a feldspathic porcelain with a coefficient of thermal expansion compatible with that of zirconia. It should be noted that the specimens in HP group were heated in the process of porcelain baking, whereas the specimens in HC group were not heated. Therefore, recovery of the primary bond strength in monolithic zirconia crowns after repair with porcelain may be attributed to the reversal of phase transformation caused by sandblasting in the process of feldspathic porcelain baking.,In the present study, one type of load was applied along the longitudinal axis to cause fracture. However, dental ceramics are often degraded as the result of multiple loading cycles or accumulation of stress-related or water-related defects., Furthermore, storage of specimens in a wet environment for simulation of oral environment may accelerate ceramic fatigue.
| Conclusion|| |
Within the limitations of this in vitro study, it may be concluded that preparation of implant-supported cement-retained monolithic zirconia crowns following abutment screw loosening necessitating restoration retrieval, and subsequent repair of the cavity with composite resin significantly decreases the fracture strength. However, in case of repair with porcelain, the eventual fracture strength value would be comparable to that of the control group.
Financial support and sponsorship
This work was supported by Dental Research Center Dentistry Research Institute of Guilan University of Medical Sciences, Guilan, Iran (grant # IR.GUMS.REC.1398.093).
Conflicts of interest
There are no conflicts of interest.
| References|| |
Al‐Aali KA, ArRejaie AS, Alrahlah A, AlFawaz YF, Abduljabbar T, Vohra F. Clinical and radiographic peri‐implant health status around narrow diameter implant‐supported single and splinted crowns. Clin Implant Dent Relat Res 2019;21:386-90.
Chrcanovic BR, Kisch J, Larsson C. Retrospective clinical evaluation of 2‐ to 6‐unit implant‐supported fixed partial dentures: mean follow‐up of 9 years. Clin Implant Dent Relat Res 2020;22:201-12.
Huang Y, Wang J. Mechanism of and factors associated with the loosening of the implant abutment screw: a review. J Esthet Restor Dent 2019;31:338-45.
Katsavochristou A, Koumoulis D. Incidence of abutment screw failure of single or splinted implant prostheses: a review and update on current clinical status. J Oral Rehabil 2019;46:776-86.
Gaddale R, Mishra SK, Chowdhary R. Complications of screw- and cement-retained implant-supported full-arch restorations: a systematic review and meta-analysis. Int J Oral Implantol 2020;13:11-40.
Rosa L, Borba M, Mallmann F, Fornari F, Bona A. Influences of screw access hole and mechanical cycling on the fracture load of implant-supported crowns. Int J Prosthodont 2019;32:423-9.
Krishnan V, Thomas CT, Sabu I. Management of abutment screw loosening: review of literature and report of a case. J Indian Prosthodont Soc 2014;14:208-14.
Patil PG. A technique for repairing a loosening abutment screw for a cement‐retained implant prosthesis. J Prosthodont 2011;20:652-5.
Mokhtarpour H, Ashtiani RE, Mahshid M, Tabatabaian F, Alikhasi M. Effect of screw access hole preparation on fracture load of implant-supported zirconia-based crowns: an in vitro study. J Dent Res Dent Clin Dent Prospects 2016;10:181-8.
Hussien ANM, Rayyan MM, Sayed NM, Segaan LG, Goodacre CJ, Kattadiyil MT. Effect of screw-access channels on the fracture resistance of 3 types of ceramic implant-supported crowns. J Prosthet Dent 2016;116:214-20.
Arami S, Tabatabaei MH, Namdar F, Safavi N, Chiniforush N. Shear bond strength of the repair composite resin to zirconia ceramic by different surface treatment. J Lasers Med Sci 2014;5:171.
Moráguez OD, Belser UC. The use of polytetrafluoroethylene tape for the management of screw access channels in implant-supported prostheses. J Prosthet Dent 2010;103:189-91.
Barragan G, Chasqueira F, Arantes-Oliveira S, Portugal J. Ceramic repair: influence of chemical and mechanical surface conditioning on adhesion to zirconia. Oral Health Dent Manag 2014;13:155-8.
Linkevicius T, Vindasiute E, Puisys A, Linkeviciene L, Svediene O. Influence of the temperature on the cement disintegration in cement-retained implant restorations. Stomatologija 2012;14:114-7.
Guazzato M, Albakry M, Ringer SP, Swain MV. Strength, fracture toughness and microstructure of a selection of all-ceramic materials. Part II. Zirconia-based dental ceramics. Dent Mater 2004;20:449-56.
Hamid Neshandar A, Mehran F, Samiye R, Hamidreza A, Zoheir M. Abutment screw loosening in single implant restorations: evaluation of fracture strength of implant-supported cement-retained monolithic zirconia restorations repaired with porcelain and composite resin. 2021.
Wood KC, Berzins DW, Luo Q, Thompson GA, Toth JM, Nagy WW. Resistance to fracture of two all-ceramic crown materials following endodontic access. J Prosthet Dent 2006;95:33-41.
Scioscia A, Helfers A, Soliman S, Krastl G, Zitzmann N. Performance of monolithic and veneered zirconia crowns after endodontic treatment and different repair strategies. Oper Dent 2018;43:170-9.
Asli HN, Rahimabadi S, Falahchai M. Flexural strength of monolithic zirconia after different surface treatments. Space 2019;3:8-11.
Curtis AR, Wright AJ, Fleming GJ. The influence of simulated masticatory loading regimes on the bi-axial flexure strength and reliability of a Y-TZP dental ceramic. J Dent 2006;34:317-25.
Ghaffari T, Moslehifard E, Motiei M. Effect of thermal and mechanical cycles on shear bond strength of zirconia core to porcelain veneer under different surface treatments. J Dent Res Dent Clin Dent Prospects 2019;13:227-33.
Tian Y, Tang S, Zheng D, Zhang Z, Ding N, Li Y. In situ synthesized particulates on a zirconia ceramic surface and their effect on bonding to porcelain. Int J Prosthodont 2021;34:463-72.
Ji M-K, Lee J-T, Yim E-K, Park C, Moon B-K, Lim H-P. Effect of atmospheric pressure plasma treatment on shear bond strength between zirconia and dental porcelain veneer. J Nanosci Nanotechnol 2020;20:5683-5.
Guess PC, Kuliš A, Witkowski S, Wolkewitz M, Zhang Y, Strub JR. Shear bond strengths between different zirconia cores and veneering ceramics and their susceptibility to thermocycling. Dent Mater 2008;24:1556-67.
Geminiani A, Chochlidakis K, Hosney S, Corsentino G, Ercoli C. Effect of framework design and firing cycle on the success rate of bilayered zirconia crowns. Quintessence Int 2019;50:30-9.
Mahgoli H, Allahyari S. Comparison between different veneering methods on failure of zirconia restorations: a review. Res J Dent Med 2018;31:58-63.
Jung Y-G., Peterson I, Kim DK, Lawn BR. Lifetime-limiting strength degradation from contact fatigue in dental ceramics. J Dent Res 2000;79:722-31.
Guazzato M, Quach L, Albakry M, Swain MV. Influence of surface and heat treatments on the flexural strength of Y-TZP dental ceramic. J Dent 2005;33:9-18.